Source: https://www.law.cornell.edu/cfr/text/16/1610.7
Timestamp: 2020-05-27 16:30:29
Document Index: 630302684

Matched Legal Cases: ['§ 1610', '§ 1610', '§ 1610', '§ 1610', '§ 1610', '§ 1610', '§ 1610', '§ 1610', '§ 1610', '§ 1610', '§ 1610', '§ 1610', '§ 1610', '§ 1610']

16 CFR § 1610.7 - Test sequence and classification criteria. | CFR | US Law | LII / Legal Information Institute
Section 1610.7. Test sequence and classification criteria.
16 CFR § 1610.7 - Test sequence and classification criteria.
§ 1610.7 Test sequence and classification criteria.
(i) Conduct preliminary tests in accordance with § 1610.6(a)(2)(i) to determine the fastest burning direction of the fabric.
(ii) Prepare and test five specimens from the fastest burning direction. The burn times determine whether to assign the preliminary classification and proceed to § 1610.6(b) or to test five additional specimens.
(iii) Assign the preliminary classification of Class 1, Normal Flammability and proceed to § 1610.6(b) when:
(B) Assign the preliminary classification of Class 1, Normal Flammability and proceed to § 1610.6(b) when there are two or more burn times with an average burn time of 3.5 seconds or greater.
(2) Step 2, Plain Surface Textile Fabrics after refurbishing in accordance with § 1610.6(b)(1).
(i) Determine the area to be most flammable per § 1610.6(a)(3)(i).
(ii) Prepare and test five specimens from the most flammable area. The burn times and visual observations determine whether to assign a preliminary classification and proceed to § 1610.6(b) or to test five additional specimens.
(iii) Assign the preliminary classification and proceed to § 1610.6(b) when:
(B) Assign the preliminary classification and continue on to § 1610.6(b) when:
(4) Step 2, Raised Surface Textile Fabric After Refurbishing in accordance with § 1610.6(b).
(i) Determine the area to be most flammable in accordance with § 1610.6(a)(3)(i).